Descripción: visita HTTP://WWW.PUBLIMAKE.COM encontraras cursos de idiomas, patron de embarcaciones, musica, videos, noticias mundiales, enlaces interesantes. Buscador de ofertas organizadas por materias y much...
3983 en - 05.2008 / c e nt be s us t al m r u m a n e n d us e This o the t J1 R 449 X2 Z1 X1 Z2 E+ Et (12V - 10A) + Isolated DC power supply ~ 10 ohms Exciter field VOLTAGE REGULATOR …Full description
Standard Specification for Zinc-Coated (Galvanized) Steel Bars for Concrete Reinforcement
A 29 - A 29M - 03 _QTI5LTAZFull description
ASTM A 123AFull description
ASTM for piping designFull description
Standard Specification for Carbon Steel Bolts, Studs, and Threaded Rod 60 000psi Tensile Strength
Especificación Normalizada para Barras de Acero de Baja Aleación Lisas y Corrugadas para Refuerzo de ConcretoDescripción completa
Norma ASTM caracterización materiales A 573.
ASTM A 123
Designation: A 449 – 04b
Standard Speciﬁcation for
Hex Cap Screws, Bolts and Studs, Steel, Heat Treated, 120/ 105/90 ksi Minimum Tensile Strength, General Use 1 This standard is issued under the ﬁxed designation A 449; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A superscript supers cript epsilon (e) indicates an editorial change since the last revision or reapproval. This standard has been approved for use by agencies of the Department of Defense.
1. Scope Scope* *
Iron and Steel Hardware A 563 Speciﬁcation for Carbon and Alloy Steel Nuts A 751 Test Test Met Methods hods,, Pra Practi ctices ces,, and Term ermino inolog logy y for Chemical Analysis of Steel Products B 695 Speci Speciﬁca ﬁcatio tion n for Coa Coatin tings gs of Zin Zincc Mec Mechan hanica ically lly Deposited on Iron and Steel D 3951 Practice for Commercial Packaging F 436 Speciﬁcation for Hardened Steel Washers F 606 Test Methods for Determining the Mechanical Properties erti es of Exter Externally nally and Inte Internall rnally y Threa Threaded ded Fast Fasteners eners,, Washers, and Rivets F 788/F 788M Speciﬁcation for Surface Discontinuities of Bolts, Screws, and Studs, Inch and Metric Series F 1470 Guide for Fastener Sampling for Speciﬁed Mechanical Properties and Performance Inspection F 1789 Terminology for F16 Mechanical Fasteners F 1941 Speciﬁcat Speciﬁcation ion for Elec Electrod trodepos eposited ited Coat Coatings ings on Thread Thr eaded ed Fas Fasten teners ers (Un (Uniﬁe iﬁed d Inc Inch h Scr Screw ew Thr Thread eadss (UN (UN/ / UNR)) Standards:4 2.2 ANSI/ASME Standards: B 1.1 Uniﬁe Uniﬁed d Screw Threads B 18.2.1 Squar Squaree and Hex Bolts Bolts and and Screws Screws B 18.24.1 18.24.1 Part Identifyin Identifying g Numb Number er (PIN) Code System
1.1 This speciﬁcat speciﬁcation ion2 covers quenched and tempered steel hex cap scre screws, ws, bolts, and stud studss havi having ng a mini minimum mum tensile tensile strength of 120 ksi for diameters 1.0 in. and smaller; 105 ksi for diameters over 1.0 in. to 1 1 ⁄ 2 in.; and 90 ksi for diameters 1 3 ⁄ 4 in. to 3.0 in. inclusive. The term fasteners in this speciﬁcation denotes hex cap screws, bolts, and studs. 1.2 The fasteners fasteners are inten intended ded for gener general al engineering engineering use. 1.3 The fasteners fasteners are furnished furnished in diam diameter eterss 1 ⁄ 4 to 3.0 in. inclus inc lusive ive.. The They y are des design ignate ated d by typ typee den denoti oting ng che chemic mical al composition as follows: 9
Typ ype eI
Plain Plai n ca carb rbon on st stee eel, l, ca carb rbon on bo boro ron n st stee eel, l, al allo loy y steel, or alloy boron steel Withdrawn 2003
1.4 Terms used in this speciﬁcati speciﬁcation on are deﬁned in Termi ermi-nology F nology F 1789 1789 unless otherwise deﬁned in this speciﬁcation. 1.5 The values stated in in inch-pound units are to be regarded as the standard. The values given in parentheses are provided for information purposes only. standard d doe doess not purport purport to add addre ress ss all of the 1.6 This standar safe sa fety ty co conc ncer erns ns,, if an anyy, as asso soci ciat ated ed wit with h its us use. e. It is th thee responsibility of the user of this standard to establish appro priate safety and health practices and determine the applicability of regulatory limitations prior to use.
3. Ordering Information Information 3.1 Order Orderss for fasteners fasteners under this speciﬁcation speciﬁcation shall include the following: 3.1.1 Quant Quantity ity (number (number of piec pieces), es), 3.1.2 Size, including including nominal diameter diameter and lengt length, h, 3.1.3 Name of product, product, 3.1.4 Type, that is, Type Type 1, 3.1.5 ASTM designatio designation n and year of issue, and 3.1.6 3.1 .6 Oth Other er com compon ponent entss suc such h as nut nutss and washers washers if required 3.1.7 Hot-Dip or Mechanically Deposited Zinc Coatings— For hot-dip or mechanically deposited zinc coatings covered by 5.1 and requiring over-tapped nuts, specify the zinc coating process required, that is, hot-dip, mechanically deposited, or no preference (see 5.1 5.1). ).
2. Referenced Documents 2.1 ASTM Standards: 3 A 153/A 153M Speciﬁcation for Zinc Coating (Hot-Dip) on
Thiss spec Thi speciﬁca iﬁcatio tion n is und under er the juri jurisdi sdictio ction n of ASTM Com Commit mittee tee F16 on Fasteners and is the direct responsibility of Subcommittee F16.02 on Steel Bolts, Nuts, Rivets, and Washers. Currentt edition approved Curren approved Nov Nov.. 1, 2004 2004.. Publis Published hed February 2005. Origin Originally ally approved in 1963. Last previous edition approved in 2004 as A 449 – 04a. 2 For ASME Boiler and Pressure Vessel Code applications see related Speciﬁcations SA-449 in Section II of that Code. 3 For referenced ASTM standards, visit the ASTM website, www.astm.org, or contact ASTM Customer Service at service@ [email protected] astm.org. g. For For Annual Annual Book of ASTM Standards volume information, refer to the standard’s Document Summary page on the ASTM website website..
Available from American Society of Mechanical Engineers (ASME), ASME International Headquarters, Three Park Ave., New York, NY 10016-5990.
A 449 – 04b 3.1.8 Other Coatings—Specify other protective coating if required (see 5.2). 3.1.9 Specify if inspection at point of manufacture is required. 3.1.10 Test reports if required. 3.1.11 Supplementary or special requirements. 3.1.12 For establishment of a part identifying system, see ASME B 18.24.1.
5.1.3 When mechanically deposited is speciﬁed, the fasteners shall be zinc coated by the mechanical deposition process in accordance with the requirements of Class 50 of Speciﬁcation B 695. 5.1.4 When no preference is speciﬁed, the supplier may furnish either a hot-dip zinc coating in accordance with Speciﬁcation A 153/A 153M, Class C, or a mechanically deposited zinc coating in accordance with Speciﬁcation B 695, Class 50. Threaded components (bolts and nuts) shall be coated by the same zinc coating process, and the suppliers’ option shall be limited to one process per item with no mixed processes in a lot.
NOTE 1—A typical ordering description follows: 1000 pieces 1 ⁄ 8 in. diameter 3 4.0 in. long hex cap screw, Type 1, ASTM A 449–XX, each with one ﬁnished hex nut ASTM A 563, Grade DH. Each component mechanically zinc coated in accordance with B 695, Class 5, Type II.
NOTE 2—When the intended application requires that assembled tension exceeds 50 % of minimum bolt or stud proof load, an anti-galling lubricant may be needed. Application of such a lubricant to nuts and a test of the lubricant efficiency are provided in Supplementary Requirement S1 of Speciﬁcation A 563 and should be speciﬁed when required.
3.2 Suitable Nuts and Washers: 3.2.1 Suitable nuts are covered in Speciﬁcation A 563. Unless otherwise speciﬁed, the grade and style of nut shall be as follows: Fastener Size and Surface Finish ⁄ 4 to 11 ⁄ 2 in., plain (or with a coating of insufficient thickness to require over-tapped nuts) Over 11 ⁄ 2 to 3 in., plain (or with a coating of insufficient thickness to require over-tapped nuts) 1 ⁄ 4 to 3 in., zinc-coated (or with a coating thickness requiring over-tapped nuts) 1
5.2 Other Coatings: 5.2.1 When other coatings are required, the purchaser shall specify the coating speciﬁcation, including the classiﬁcation codes or grade numbers to identify the coating material, thickness, supplemental treatments, or other requirements to deﬁne the coating. The fasteners shall be coated in accordance with and conform to the speciﬁed coating speciﬁcation. 5.2.2 When a speciﬁcation does not apply, the purchaser shall specify the desired coating, coating thickness, supplemental treatments, or other requirements to deﬁne the coating.
Nut Grade and Style A B, hex A, heavy hex DH, heavy hex
Nuts of other grades and styles having speciﬁed proof load stresses (Speciﬁcation A 563, Table 3) greater than the speciﬁed grade and style of nut are suitable.
3.2.2 Unless otherwise speciﬁed, washers ordered with fasteners shall be furnished to the requirements of Speciﬁcation F 436, Type 1.
6. Chemical Composition 6.1 Type 1 fasteners shall be plain carbon steel, carbon boron steel, alloy steel, or alloy boron steels, at the manufacturers option, conforming to the requirements in Table 1. 6.2 Product analyses made on ﬁnished fasteners representing each lot shall conform to the product analysis requirements speciﬁed in Table 1, as applicable. 6.3 Heats of steel to which bismuth, selenium, tellurium, or lead has been intentionally added shall not be permitted for bolts. Compliance shall be based on certiﬁcation that heats of steel having any of the listed elements intentionally added were not used to produce the bolts. 6.4 Chemical analyses shall be performed in accordance with Test Methods, Practices, and Terminology A 751.
4. Materials and Manufacture 4.1 Heat Treatment : 4.1.1 Type 1 fasteners produced from medium carbon steel shall be quenched in a liquid medium from the austenitizing temperature. 4.1.2 Type 1 fasteners produced from medium carbon steel to which chromium, nickel, molybdenum, or boron were intentionally added shall be quenched in oil from the austenitizing temperature. 4.1.3 Type 1 fasteners, regardless of the steel used, shall be tempered by reheating to not less than 800°F. 4.2 Threading—Threads shall be rolled, cut, or ground. 4.3 Secondary Processing —If any processing which can affect the mechanical properties of the fasteners is performed after the initial testing, the fasteners shall be retested for all speciﬁed mechanical properties affected by the reprocessing.
7. Mechanical Properties 7.1 Hardness—The fasteners shall conform to the hardness speciﬁed in Table 2. See Table 2, Note A. 7.2 Tensile Properties: 7.2.1 Except as permitted in 7.2.2 for long fasteners and 7.2.3 for short fasteners, hex cap screws and hex and square head bolts in sizes 1.00 in. and smaller having a length of 2 1 ⁄ 4 D and longer and sizes 1 1 ⁄ 8 to 11 ⁄ 2 in. inclusive having a length of 3D and longer shall be wedge tested full size. Bolts with heads other than hex or square shall be axially tested. Both wedge and axially tested hex cap screws and bolts shall conform to the proof load or alternative proof load, and minimum wedge tensile load in Tables 3 and 4, as applicable. The load applied during proof load testing shall be equal to or greater than the proof load in Table 3 or Table 4 as applicable.
5. Protective Coatings 5.1 Zinc, Hot Dip, and Mechanically Deposited Requiring Over-tapped Nuts: 5.1.1 When zinc-coated fasteners are required, the purchaser shall specify the zinc-coating process, such as, hot-dip, mechanically deposited, or no preference. 5.1.2 When hot dip is speciﬁed, the fasteners shall be zinc coated by the hot-dip process in accordance with the requirements of Class C of Speciﬁcation A 153/A 153M. 2
A 449 – 04b TABLE 1 Chemical Requirements for Type 1 Fasteners Element Carbon Manganese, min Phosphorus, max Sulfur, max Silicon Element Carbon Manganese, min Phosphorus, max Sulfur, max Silicon Boron Element Carbon Manganese, min Phosphorus, max Sulfur, max Silicon Alloying Elements Element Carbon Manganese, min Phosphorus, max Sulfur, max Silicon Boron Alloying Elements
the studs are too long for full size testing, machined specimens shall be tested and shall conform to the tensile requirements in Table 5. 7.2.5 If fasteners are subjected to both hardness and tensile tests, the tensile test results shall take precedence in the event of low hardness test results. 7.2.6 If fasteners are subjected to both full size and machined specimen tests, the full size test results shall take precedence if the results of the two methods differ.
Carbon Steel Heat Analysis
0.30–0.52 0.60 0.040 0.050 0.015–0.30
0.28–0.55 0.57 0.048 0.058 0.13–0.32 Carbon Steel
0.30–0.52 0.60 0.040 0.050 0.10–0.30 0.0005–0.003
0.28–0.55 0.57 0.048 0.058 0.08–0.32 0.0005–0.003
8. Dimensions 8.1 Head and Body : 8.1.1 Hex Cap Screws —Unless otherwise speciﬁed, hex cap screws shall be furnished with dimensions conforming to ASME B 18.2.1. 8.1.2 Bolts—When styles other than speciﬁed in 8.1.1 are required, they shall have dimensions conforming to those speciﬁed by the purchaser. 8.1.3 Studs—Studs shall have dimensions conforming to those speciﬁed by the purchaser. 8.2 Threads: 8.2.1 Uncoated — Unless otherwise speciﬁed, uncoated threads shall be the Uniﬁed Coarse Thread Series as speciﬁed in the latest issue of ASME B 1.1, and shall have Class 2A tolerances. 8.2.2 Coated —Unless otherwise speciﬁed, zinc-coated bolts, to be used with zinc-coated nuts or tapped holes, which are tapped oversize in accordance with Speciﬁcation A 563, shall have UNC Class 2A threads before hot-dip or mechanically deposited zinc-coating. After zinc coating, the pitch diameter and major diameter shall not exceed the Class 2A limits by more than the following amounts:
Carbon Steel Heat Analysis
0.30–0.52 0.60 0.035 0.040 0.15–0.35
0.28–0.55 0.57 0.040 0.045 0.13–0.37
Carbon Steel Heat Analysis
0.30–0.52 0.60 0.035 0.040 0.15–0.35 0.0005–0.003
0.28–0.55 0.57 0.040 0.045 0.13–0.37 0.0005–0.003
Steel, as deﬁned by the American Iron and Steel Institute, shall be considered to be alloy when the maximum of the range given for the content of alloying elements exceeds one or more of the following limits: manganese, 1.65 %; silicon, 0.60 %; copper, 0.60 % or in which a deﬁnite range or a deﬁnite minimum quantity of any of the following elements is speciﬁed or required within the limits of the recognized ﬁeld of constructional alloy steels: aluminum, chromium up to 3.99 %, cobalt, columbium, molybdenum, nickel, titanium, tungsten, vanadium, zirconium, or any other alloying elements added to obtain a desired alloying effect.
7.2.2 Hex cap screws and square head bolts larger than 1 1 ⁄ 2 in. diameter, other than those excepted in 7.2.3, shall preferably be tested full size and when so tested shall conform to the tensile strength and either the speciﬁed proof load or yield strength requirements in Tables 3 and 4, as applicable. When equipment of sufficient capacity for full size testing is not available, or when the length of the bolt makes full size testing impractical, machined specimens shall be tested and shall conform to the requirements of Table 5. 7.2.3 Sizes 1.00 in. and smaller having a length shorter than 21 ⁄ 4 D down to 2D inclusive, which cannot be wedge tensile tested shall be axially tension tested full size and shall conform to the minimum tensile load and proof load or alternate proof load speciﬁed in Tables 3 and 4. Sizes 1.00 in. and smaller having a length shorter than 2D which cannot be axially tensile tested shall be qualiﬁed on the basis of hardness. 7.2.4 Studs 3D and longer shall be axially tension tested full size and shall conform to the tensile and proof load or alternate proof load speciﬁed in Table 3 and Table 4, as applicable. When equipment for full size testing is not available, or when
Oversize Limit, in. A Hot-Dip Zinc
0.016 0.017 0.018 0.020 0.022 0.024 0.027 0.050
0.012 0.012 0.012 0.013 0.015 0.016 0.018 0.033
A Hot-dip zinc nuts are tapped oversize after coating and mechanical zinc coated nuts are tapped oversize before coating.
8.2.3 Unless otherwise speciﬁed, fasteners electroplated or mechanically coated to 0.0005 in. or less, threads prior to plating shall conform to ASME B 1.1 Class 2A and after plating shall not exceed the Class 3A maximum limits, that is, Class 2A plus the allowance. 9. Workmanship, Finish, and Appearance 9.1 Surface discontinuity limits, inspection, and evaluation shall be in accordance with Speciﬁcation F 788/F 788M. 10. Number of Tests and Retests 10.1 Testing Responsibility: 10.1.1 Each lot shall be tested by the manufacturer prior to shipment in accordance with the lot identiﬁcation control quality assurance plan in 10.2-10.5. 3
A 449 – 04b TABLE 2 Hardness Requirements for Hex Cap Screws, Bolts, and Studs Nominal Diameter, in.
Length, in. A
⁄ 4 to 1, inclusive
Less than 2D 2D and over Less than 3DA 3D and over Less than 3D A 3D and over
Over 1 to 11 ⁄ 2 , inclusive Over 11 ⁄ 2 to 3, inclusive
253 ... 223 ... 183 ...
319 319 286 286 235 235
25 ... 19 ... ... ...
34 34 30 30 ... ...
Hex cap screws and bolts larger than 1.00 in. diameter and shorter than 3D and all studs shorter than 3D are subject only to minimum and maximum hardness. D = Nominal diameter or thread size
TABLE 3 Tensile Load Requirements for Coarse-Thread Full-Size Hex Cap Screws, Bolts and Studs Bolt or Stud Diameter, in.
Threads per in.A
Stress Area,B in.2
Tensile Load, min, lbf C
Proof Load, Length Measurement Method, lbf C
Alternative Proof Load, Yield Strength Method (0.2 % Offset), lbf C
⁄ 4 ⁄ 16 3 ⁄ 8
20 18 16
0.0318 0.0524 0.0775
3 800 6 300 9 300
2 700 4 450 6 600
2 900 4 800 7 100
⁄ 16 1 ⁄ 2 9 ⁄ 16
14 13 12
0.1063 0.1419 0.182
12 750 17 050 21 850
9 050 12 050 15 450
9 800 13 050 16 750
⁄ 8 ⁄ 4 7 ⁄ 8
11 10 9
0.226 0.334 0.462
27 100 40 100 55 450
19 200 28 400 39 250
20 800 30 700 42 500
1 11 ⁄ 8 11 ⁄ 4
8 7 7
0.606 0.763 0.969
72 700 80 100 101 700
51 500 56 450 71 700
55 750 61 800 78 500
13 ⁄ 8 11 ⁄ 2 13 ⁄ 4
6 6 5
1.155 1.405 1.90
121 300 147 500 171 000
85 450 104 000 104 500
93 550 113 800 110 200
2 21 ⁄ 4 21 ⁄ 2
41 ⁄ 2 41 ⁄ 2 4
2.50 3.25 4.00
225 000 292 500 360 000
137 500 178 750 220 000
145 000 188 500 232 000
23 ⁄ 4 3
443 700 537 300
271 150 328 350
286 000 346 200
For 8 threads per in., sizes 1 1 ⁄ 8 to 1 1 ⁄ 2 in., inclusive, stresses of 105 000 psi, 74 000 psi, and 81 000 psi shall be used for calculating the values in columns 4, 5, and 6 respectively. B The stress area is taken from ASME B1.1 which uses the equation below to calculate the values: As = 0.7854[ D − (0.9743/ n) ]2 where: As = stress area, D = nominal diameter, and n = threads per in. C Values tabulated are based on the following: Bolt Size, in. ⁄ 4 to 1, incl. 11 ⁄ 8 to 11 ⁄ 2 , incl. 13 ⁄ 4 to 3, incl. 1
Column 4, psi
Column 5, psi
Column 6, psi
120 000 105 000 90 000
85 000 74 000 55 000
92 000 81 000 58 000
10.1.2 When fasteners are furnished by a source other than the manufacturer, the responsible party as deﬁned in 15.1 shall be responsible for assuring all tests have been performed and the fasteners comply with the requirements of this speciﬁcation (see 4.3). 10.2 Purpose of Lot Inspection—The purpose of a lot inspection program is to ensure that each lot conforms to the requirements of this speciﬁcation. For such a plan to be fully
effective, it is essential that secondary processors, distributors, and purchasers maintain the identiﬁcation and integrity of each lot until the product is installed. 10.3 Lot Processing—All fasteners shall be processed in accordance with a lot identiﬁcation-control quality assurance plan. The manufacturer, secondary processors, and distributors shall identify and maintain the integrity of each lot from raw material selection through all operations and treatments to ﬁnal
A 449 – 04b TABLE 4 Tensile Load Requirements for Fine-Thread Full-Size Hex Cap Screws, Bolts, and Studs Bolt or Stud Diameter, in.
Threads per in.
Stress Area,A in.2
Tensile Load, min, lbf B
Proof Load, Length Measurement Method, lbf B
Alternative Proof Load, Yield Strength Method (0.2 % Offset), min, lbf B
⁄ 4 ⁄ 16 3 ⁄ 8
28 24 24
0.0364 0.0580 0.0878
4 350 6 950 10 550
3 100 4 950 7 450
3 500 5 350 8 100
⁄ 16 ⁄ 2 9 ⁄ 16
20 20 18
0.1187 0.1599 0.203
14 250 19 200 24 350
10 100 13 600 17 250
10 900 14 700 18 700
⁄ 8 ⁄ 4 7 ⁄ 8
18 16 14
0.256 0.373 0.509
30 700 44 750 61 100
21 750 31 700 43 250
23 500 34 300 46 800
1 11 ⁄ 8 11 ⁄ 4
12 12 12
0.663 0.856 1.073
79 550 89 900 112 650
56 350 63 350 79 400
61 000 69 350 86 900
13 ⁄ 8 11 ⁄ 2
138 100 166 000
97 300 117 000
106 500 128 000
See footnote B in Table 3. See footnote C in Table 3.
TABLE 5 Tensile Strength Requirements for Specimens Machined from Hex Cap Screws, Bolts, and Studs Nominal Diameter, in. ⁄ 4 to 1, incl. Over 1 to 11 ⁄ 2 , incl. Over 11 ⁄ 2 to 3, incl. 1
Tensile Strength, min, psi
Yield Strength, min, psi
Elongation in 4D , min, %
Reduction of Area, min, %
120 000 105 000 90 000
92 000 81 000 58 000
14 14 14
35 35 35
testing method of full size product method or the machined test specimens method depending on size and length as speciﬁed in 7.2.2-7.2.6. Bolts with heads other than hex or square shall be axially tested. Fracture on full size tests shall be in the body or threads of the fastener without a fracture at the junction of the head and body. 11.3 Studs shall be tested by the axial tension method as described in the second paragraph of axial tension testing of full size products in the Test Methods section of Test Methods F 606.
packing and shipment. Each lot shall be assigned its own lot-identiﬁcation number, each lot shall be tested, and the inspection test reports for each lot shall be retained. 10.4 Lot Deﬁnition: 10.4.1 Standard Lot —A lot shall be a quantity of uniquely identiﬁed fasteners of the same nominal size and length produced consecutively at the initial operation from a single mill heat of material and processed at one time, by the same processor in the same manner so that statistical sampling is valid. The identity of the lot and lot integrity shall be maintained throughout all subsequent operations and packaging. 10.5 Number of Tests — The minimum number of tests from each lot for the tests speciﬁed below shall be as follows: Tests
Hardness, tensile strength, proof load and rotational capacity Coating weight/thickness Surface discontinuities Dimensions and thread ﬁt A
11.4 Proof load shall be determined using Method 1, length measurement, or Method 2, yield strength, at the option of the manufacturer. 12. Inspection 12.1 If the inspection described in 12.2 is required by the purchaser, it shall be speciﬁed in the inquiry and contract or order. 12.2 The purchaser’s representative shall have free entry to all parts of the manufacturer’s works or supplier’s place of business that concern the manufacture or supply of the fasteners. The manufacturer shall afford the purchaser’s representative all reasonable facilities to satisfy him that the fasteners are being furnished in accordance with this speciﬁcation. All tests and inspections required by the speciﬁcation that are requested by the purchaser’s representative shall be made before shipment, and shall be conducted as not to interfere unnecessarily with the operation of the manufacturer’s works or supplier’s place of business.
Number of Tests in Accordance With Guide F 1470 The referenced coating speciﬁcationA Speciﬁcation F 788/F 788M ASME B 18.2.1
Guide F 1470 if the coating speciﬁcation does not specify a testing frequency.
11. Test Methods
13. Rejection and Rehearing
11.1 Tensile, proof load, and hardness tests shall be conducted in accordance with Test Methods F 606. 11.2 Tensile strength for hex cap screws and hex and square bolts shall be determined using the wedge or axial tension
13.1 Disposition of nonconforming fasteners shall be in accordance with the section on Disposition of Nonconforming Lots of Guide F 1470. 5
A 449 – 04b 14. Certiﬁcation
addition to the A 449 marking, fasteners shall be permitted to be marked with three radial lines 120° apart. 16.3 Marking Location and Methods: 16.3.1 All markings shall be located on the top of a hex cap screw and bolt heads and on one end of studs and shall be either raised or depressed at the manufacturer’s option. 16.3.2 Type and manufacturer’s or private label distributor’s identiﬁcation shall be separate and distinct. The two identiﬁcations shall preferably be in different locations and, when on the same level, shall be separated by at least two spaces. 16.4 Acceptance Criteria—Fasteners which are not marked in accordance with these provisions shall be considered nonconforming and subject to rejection.
14.1 When speciﬁed on the purchase order, the manufacturer or supplier, whichever is the responsible party as deﬁned in Section 15, shall furnish the purchaser test reports which include the following: 14.1.1 Heat analysis, heat number, and a statement certifying that heats having the elements listed in 6.3 intentionally added were not used to produce the fasteners, 14.1.2 Results of hardness, tensile, and proof load tests, 14.1.3 Zinc coating measured coating weight/thickness for coated fasteners, 14.1.4 Statement of compliance with dimensional and thread ﬁt requirements, 14.1.5 Lot number and purchase order number, 14.1.6 Complete mailing address of responsible party, and 14.1.7 Title and signature of the individual assigned certiﬁcation responsibility by the company officers. 14.2 Failure to include all the required information on the test report shall be cause for rejection.
17. Packaging and Package Marking 17.1 Packaging: 17.1.1 Unless otherwise speciﬁed, packaging shall be in accordance with Practice D 3951. 17.1.2 When special packaging requirements are required, they shall be deﬁned at the time of the inquiry and order. 17.2 Package Marking : 17.2.1 Each shipping unit shall include or be plainly marked with the following information: 18.104.22.168 ASTM designation and type, 22.214.171.124 Size, 126.96.36.199 Name and brand or trademark of the manufacturer, 188.8.131.52 Number of pieces, 184.108.40.206 Lot number, 220.127.116.11 Purchase order number, and 18.104.22.168 Country of origin.
15. Responsibility 15.1 The party responsible for the fastener shall be the organization that supplies the fastener to the purchaser. 16. Product Marking 16.1 Manufacturers Identiﬁcation—All hex cap screws and bolts and one end of studs 3 ⁄ 8 in. and larger, and whenever feasible studs smaller than 3 ⁄ 8 in., shall be marked by the manufacturer with a unique identiﬁer to identify the manufacturer or private label distributor, as appropriate. 16.2 Type Identiﬁcation—Type 1 hex cap screws and bolts and one end of Type 1 studs 3 ⁄ 8 in. and larger, and whenever feasible studs smaller than 3 ⁄ 8 in., shall be marked “A 449.” In
S1.2 Marking small sizes (customarily less than 0.375 in.) may not be practical. Consult the producer for the minimum size that can be marked.
S1.1 Studs that are continuously threaded with the same class of thread shall be marked on each end with the marking required by Section 16.
SUMMARY OF CHANGES Committee F16 has identiﬁed the location of selected changes to this standard since the last issue, A 449 – 04a, that may impact the use of this standard. (Approved Nov. 1, 2004.) (1) Clariﬁed fasteners covered throughout the speciﬁcation are hex cap screws, bolts, or other conﬁgurations as speciﬁed by the purchaser, and studs. (2) Deleted Type 2 low and medium carbon martensite steel fasteners. (3) Revised Section 3, Ordering Information. (4) In 3.2.2, speciﬁed washers ordered with fasteners be furnished as F 436, Type 1, unless otherwise speciﬁed. (5) Deleted former Section 4.1, Steelmaking Process.
(6 ) In 4.1.2, mandated alloy steels to be quenched in oil. (7 ) Added 4.3, Secondary Processing. (8) Revised Section 6, Chemical Composition, to permit carbon boron, alloy, and alloy boron steel. (9) Revised Table 2, Hardness, to specify the same limits as in A 325. (10) In 7.2.1-7.2.4, revised the wedge test and machined test specimen test break points. (11) In 7.2.3, added the requirement that hex cap screws and 6
A 449 – 04b (15) Added Section 13, Rejection and Rehearing, and invoked Guide F 1470 for disposition of nonconforming fasteners.
bolts shorter than 2 1 ⁄ 4 D down to 2D inclusive which cannot be wedge tested be axially tension tested. (12) Delete old Table 6, Sample Size for Inspection of Hot Dip or Mechanically deposited Zinc Coated Threads and the reference to MIL-STD-105. Sampling is covered in the referenced dimensional standards. (13) Revised 9.1 listing manufacturing and material defect which could make the fasteners unsuitable for the intended application and replaced with a reference to Speciﬁcation F 788/F 788M. (14) Deleted former Sections 10.1 through 10.5 covering Number of Tests and replaced them with a reference to Guide F 1470.
(16 ) Added Section 14, Certiﬁcation, on a “when speciﬁed basis.” (17 ) In 16.2, replaced three radial line marking with “A 449.” (18) In Section 7, added wording allowing machined specimens for fasteners too large for full size testing. (19) In Section 16, Product Marking, replaced the three radial lines marking with “A 449” and allowed as additional marking “three radial lines.”
Committee F16 has identiﬁed the location of selected changes to this standard since the last issue, A 449 – 04, that may impact the use of this standard. (Approved Aug. 1, 2004.) ( 1)
Revised Section 15, Responsibility.
Committee F16 has identiﬁed the location of selected changes to this standard since the last issue, A 449 – 00, that may impact the use of this standard. (Approved Jan. 1, 2004.) ( 1)
Added Section 1.7 that references Terminology F 1789. ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below. This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or firstname.lastname@example.org (e-mail); or through the ASTM website (www.astm.org).